Single-Crystal to Single-Crystal Phase Transition and Segmented Thermochromic Luminescence in a Dynamic 3D Interpenetrated Ag(I) Coordination Network.
Yan, Zhi-Hao; Li, Xiao-Yu; Liu, Li-Wei; Yu, Si-Qi; Wang, Xing-Po; Sun, Di; Inorganic chemistry 55 (2016) 1096–1101; doi:10.1021/acs.inorgchem.5b02200

data_4346828
_publ_section_title
;
 Single-Crystal to Single-Crystal Phase Transition and Segmented
 Thermochromic Luminescence in a Dynamic 3D Interpenetrated Ag(I)
 Coordination Network.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              1096
_journal_page_last               1101
_journal_paper_doi               10.1021/acs.inorgchem.5b02200
_journal_volume                  55
_journal_year                    2016
_chemical_formula_moiety         'C12 H8 Ag2 N2 O4, H2 O'
_chemical_formula_sum            'C12 H10 Ag2 N2 O5'
_chemical_formula_weight         477.96
_space_group_crystal_system      orthorhombic
_space_group_IT_number           73
_space_group_name_Hall           '-I 2b 2c'
_space_group_name_H-M_alt        'I b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            16
_cell_length_a                   7.1620(5)
_cell_length_b                   23.7651(15)
_cell_length_c                   30.7049(19)
_cell_measurement_temperature    148(2)
_cell_volume                     5226.1(6)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      148(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker Apex II'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0234
_diffrn_reflns_av_sigmaI/netI    0.0174
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       36
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            12056
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.33
_exptl_absorpt_coefficient_mu    3.020
_exptl_absorpt_correction_T_max  0.5189
_exptl_absorpt_correction_T_min  0.4643
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.430
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             3680
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.25
_refine_diff_density_max         1.237
_refine_diff_density_min         -0.903
_refine_diff_density_rms         0.122
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.323
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     190
_refine_ls_number_reflns         2315
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.323
_refine_ls_R_factor_all          0.0408
_refine_ls_R_factor_gt           0.0390
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0087P)^2^+73.8673P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0803
_refine_ls_wR_factor_ref         0.0811
_reflns_number_gt                2218
_reflns_number_total             2315
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5b02200_si_002.cif
_cod_data_source_block           p-148K
_cod_database_code               4346828